#------------------------------------------------------------------------------
#$Date: 2016-03-26 22:33:39 +0200 (Sat, 26 Mar 2016) $
#$Revision: 180510 $
#$URL: svn://www.crystallography.net/cod/cif/7/21/79/7217920.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_7217920
loop_
_publ_author_name
'Pasán, Jorge'
'Sanchiz, Joaquín'
'Fabelo, Óscar'
'Cañadillas-Delgado, Laura'
'Déniz, Mariadel'
'Díaz-Gallifa, Pau'
'Martínez-Benito, Carla'
'Lloret, Francesc'
'Julve, Miguel'
'Ruiz-Pérez, Catalina'
_publ_section_title
;
 Influence of the coligand in the magnetic properties of a series of
 copper(ii)--phenylmalonate complexes
;
_journal_issue                   35
_journal_name_full               CrystEngComm
_journal_page_first              8106
_journal_paper_doi               10.1039/C4CE00834K
_journal_volume                  16
_journal_year                    2014
_chemical_formula_sum            'C14 H10 Cl Cu N O4'
_chemical_formula_weight         355.22
_chemical_name_systematic
;
 ?
;
_space_group_crystal_system      monoclinic
_space_group_IT_number           14
_space_group_name_Hall           '-P 2yn'
_space_group_name_H-M_alt        'P 1 21/n 1'
_symmetry_space_group_name_Hall  '-P 2yn'
_symmetry_space_group_name_H-M   'P 1 21/n 1'
_atom_sites_solution_hydrogens   geom
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90
_cell_angle_beta                 93.297(13)
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   6.2264(11)
_cell_length_b                   30.6016(17)
_cell_length_c                   6.9804(12)
_cell_measurement_temperature    293(2)
_cell_volume                     1327.8(3)
_computing_cell_refinement
'Dirax/lsq (Duisenberg & Schreurs, 1989-2000)'
_computing_data_collection       'Collect (Nonius BV, 1997-2000)'
_computing_data_reduction        'EvalCCD (Duisenberg & Schreurs 1990-2000)'
_computing_molecular_graphics    CRYSTALMAKER
_computing_publication_material  'PARST97 (Nardelli, 1997)'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1997)'
_diffrn_ambient_temperature      293(2)
_diffrn_detector                 'CCD plate'
_diffrn_detector_area_resol_mean 9
_diffrn_measured_fraction_theta_full 0.970
_diffrn_measured_fraction_theta_max 0.961
_diffrn_measurement_device       '95mm CCD camera on κ-goniostat'
_diffrn_measurement_device_type  KappaCCD
_diffrn_measurement_method       'CCD rotation images, thick slices'
_diffrn_radiation_monochromator  'horizonally mounted graphite crystal'
_diffrn_radiation_probe          x-ray
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0659
_diffrn_reflns_av_unetI/netI     0.1301
_diffrn_reflns_Laue_measured_fraction_full 0.970
_diffrn_reflns_Laue_measured_fraction_max 0.961
_diffrn_reflns_limit_h_max       8
_diffrn_reflns_limit_h_min       -7
_diffrn_reflns_limit_k_max       38
_diffrn_reflns_limit_k_min       -42
_diffrn_reflns_limit_l_max       9
_diffrn_reflns_limit_l_min       -9
_diffrn_reflns_number            8791
_diffrn_reflns_point_group_measured_fraction_full 0.970
_diffrn_reflns_point_group_measured_fraction_max 0.961
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         29.999
_diffrn_reflns_theta_min         6.434
_diffrn_source                   'Enraf Nonius FR590'
_exptl_absorpt_coefficient_mu    1.860
_exptl_absorpt_correction_T_max  0.93
_exptl_absorpt_correction_T_min  0.68
_exptl_absorpt_correction_type   empirical
_exptl_absorpt_process_details
;
SADABS: Area-Detector Absorption Correction; 
Siemens Industrial Automation, Inc.: Madison, WI, 1996.
;
_exptl_crystal_colour            Blue
_exptl_crystal_density_diffrn    1.777
_exptl_crystal_description       Sheets
_exptl_crystal_F_000             716
_exptl_crystal_size_max          0.3
_exptl_crystal_size_mid          0.18
_exptl_crystal_size_min          0.04
_refine_diff_density_max         2.129
_refine_diff_density_min         -1.373
_refine_diff_density_rms         0.144
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.148
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     190
_refine_ls_number_reflns         3721
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.148
_refine_ls_R_factor_all          0.1535
_refine_ls_R_factor_gt           0.0876
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[σ²(Fo²)+(0.0388P)²+9.4418P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1791
_refine_ls_wR_factor_ref         0.1960
_reflns_Friedel_coverage         0.000
_reflns_number_gt                2168
_reflns_number_total             3721
_reflns_threshold_expression     'I > 2σ(I)'
_cod_duplicate_entry             7216201
_cod_data_source_file            c4ce00834k2.cif
_cod_data_source_block           compound_6
_cod_database_code               7217920
#BEGIN Tags that were not found in dictionaries:
_shelx_space_group_comment
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
#END Tags that were not found in dictionaries
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x+1/2, y+1/2, -z+1/2'
'-x, -y, -z'
'x-1/2, -y-1/2, z-1/2'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
C1 C 1.0900(9) 0.2866(2) 0.3632(8) 0.0174(12) Uani 1 1 d . .
C2 C 1.0026(10) 0.3087(2) 0.1752(9) 0.0183(13) Uani 1 1 d . .
H2 H 0.8466 0.3041 0.1682 0.022 Uiso 1 1 calc R U
C3 C 1.0898(9) 0.2830(2) 0.0047(8) 0.0184(13) Uani 1 1 d . .
C4 C 1.0356(11) 0.3576(2) 0.1658(9) 0.0215(14) Uani 1 1 d . .
C5 C 1.2381(13) 0.3765(2) 0.2052(10) 0.0306(17) Uani 1 1 d . .
H5 H 1.3572 0.3587 0.2325 0.037 Uiso 1 1 calc R U
C6 C 1.2620(15) 0.4211(3) 0.2037(12) 0.041(2) Uani 1 1 d . .
H6 H 1.3961 0.4336 0.2332 0.049 Uiso 1 1 calc R U
C7 C 1.0840(17) 0.4478(3) 0.1578(12) 0.044(2) Uani 1 1 d . .
H7 H 1.0993 0.4780 0.1583 0.053 Uiso 1 1 calc R U
C8 C 0.8881(16) 0.4296(3) 0.1122(12) 0.044(2) Uani 1 1 d . .
H8 H 0.7710 0.4473 0.0778 0.053 Uiso 1 1 calc R U
C9 C 0.8628(12) 0.3847(3) 0.1168(10) 0.0306(17) Uani 1 1 d . .
H9 H 0.7282 0.3725 0.0867 0.037 Uiso 1 1 calc R U
C10 C 1.2528(12) 0.1472(3) 0.1365(10) 0.0322(17) Uani 1 1 d . .
H10 H 1.3325 0.1724 0.1193 0.039 Uiso 1 1 calc R U
C11 C 1.3422(14) 0.1076(3) 0.0966(11) 0.039(2) Uani 1 1 d . .
H11 H 1.4806 0.1063 0.0534 0.047 Uiso 1 1 calc R U
C12 C 1.2272(14) 0.0698(3) 0.1205(12) 0.038(2) Uani 1 1 d . .
H12 H 1.2843 0.0426 0.0929 0.046 Uiso 1 1 calc R U
C13 C 1.0238(14) 0.0739(2) 0.1871(11) 0.0353(18) Uani 1 1 d . .
C14 C 0.9400(11) 0.1144(2) 0.2253(10) 0.0268(16) Uani 1 1 d . .
H14 H 0.8023 0.1164 0.2696 0.032 Uiso 1 1 calc R U
Cl1 Cl 0.8659(5) 0.02787(7) 0.2203(4) 0.0615(7) Uani 1 1 d . .
Cu1 Cu 0.88139(13) 0.21523(3) 0.18980(11) 0.0190(2) Uani 1 1 d . .
N1 N 1.0529(9) 0.15088(19) 0.1999(8) 0.0251(13) Uani 1 1 d . .
O1 O 1.1927(8) 0.30975(15) 0.4840(6) 0.0229(10) Uani 1 1 d . .
O4 O 1.0550(8) 0.24327(15) -0.0071(7) 0.0242(10) Uani 1 1 d . .
O2 O 1.0546(8) 0.24694(16) 0.3850(6) 0.0243(11) Uani 1 1 d . .
O3 O 1.1913(8) 0.30533(15) -0.1134(6) 0.0237(10) Uani 1 1 d . .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Cl Cl 0.1484 0.1585 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Cu Cu 0.3201 1.2651 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O2 C1 O1 123.9(6) . .
O2 C1 C2 118.3(5) . .
O1 C1 C2 117.8(6) . .
C4 C2 C1 115.3(5) . .
C4 C2 C3 114.5(5) . .
C1 C2 C3 107.9(5) . .
O4 C3 O3 125.4(6) . .
O4 C3 C2 118.8(5) . .
O3 C3 C2 115.8(6) . .
C9 C4 C5 118.6(7) . .
C9 C4 C2 119.8(6) . .
C5 C4 C2 121.6(6) . .
C6 C5 C4 120.4(7) . .
C5 C6 C7 119.8(8) . .
C8 C7 C6 120.2(8) . .
C7 C8 C9 120.2(8) . .
C8 C9 C4 120.8(8) . .
N1 C10 C11 122.3(7) . .
C10 C11 C12 119.9(8) . .
C11 C12 C13 117.4(7) . .
C14 C13 C12 120.8(7) . .
C14 C13 Cl1 118.6(6) . .
C12 C13 Cl1 120.6(6) . .
N1 C14 C13 121.2(7) . .
O2 Cu1 O1 173.0(2) . 4_565
O2 Cu1 O3 90.1(2) . 4_566
O1 Cu1 O3 91.58(19) 4_565 4_566
O2 Cu1 O4 88.1(2) . .
O1 Cu1 O4 89.3(2) 4_565 .
O3 Cu1 O4 172.8(2) 4_566 .
O2 Cu1 N1 99.9(2) . .
O1 Cu1 N1 86.8(2) 4_565 .
O3 Cu1 N1 90.1(2) 4_566 .
O4 Cu1 N1 97.1(2) . .
C14 N1 C10 118.4(6) . .
C14 N1 Cu1 119.0(5) . .
C10 N1 Cu1 120.7(5) . .
C1 O1 Cu1 122.4(4) . 4_666
C3 O4 Cu1 118.6(4) . .
C1 O2 Cu1 119.7(4) . .
C3 O3 Cu1 128.6(4) . 4_665
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
C1 O2 1.245(8) .
C1 O1 1.248(7) .
C1 C2 1.547(9) .
C2 C4 1.510(9) .
C2 C3 1.551(9) .
C3 O4 1.237(8) .
C3 O3 1.267(8) .
C4 C9 1.385(10) .
C4 C5 1.400(10) .
C5 C6 1.375(11) .
C6 C7 1.399(13) .
C7 C8 1.362(13) .
C8 C9 1.383(11) .
C10 N1 1.349(9) .
C10 C11 1.368(11) .
C11 C12 1.375(12) .
C12 C13 1.379(12) .
C13 C14 1.377(10) .
C13 Cl1 1.741(8) .
C14 N1 1.337(9) .
Cu1 O2 1.948(5) .
Cu1 O1 1.958(4) 4_565
Cu1 O3 1.967(5) 4_566
Cu1 O4 1.991(5) .
Cu1 N1 2.239(6) .
O1 Cu1 1.958(4) 4_666
O3 Cu1 1.967(5) 4_665
